Download presentation

1
WELCOME

2
**CEMENT CONCRETE MIX DESIGN**

by K. RAMESH Research Officer, Engineering Materials Laboratory, A.P. Engineering Research Laboratories, Himayatsagar, HYDERABAD

3
Cement Concrete Mix Design means, determination of the proportion of the concrete ingredients i.e. Cement, Water, Fine Aggregate,Coarse Aggregate which would produce concrete possessing specified properties such as workability, strength and durability with maximum overall economy.

4
**Methods of Concrete Mix Design**

I.S. Method British Method A.C.I. Method etc.

5
**These Methods are based on two basic assumptions**

Compressive Strength of Concrete is governed by its Water-Cement Ratio Workability of Concrete is governed by its Water Content

6
**Data required for concrete mix design**

Grade of Concrete Eg: RCC-M30-A20 Slump required in mm Eg: 25 – 75 mm Degree of Site Control Eg: Good Type of Exposure Eg: Moderate Grade of Cement Eg: OPC 43 Grade

7
**Workability (Clause 7.1, IS:456-2000) Placing Conditions**

Degree of Workability Slump (mm) 1 2 3 Blinding Concrete; Shallow Sections; Pavements using pavers Very Low See 7.1.1 Mass Concrete; Lightly reinforced sections in Slabs, Beams, Walls, Columns; Floors; Hand placed Pavements; Canal lining; Strip Footings Low 25-75 Heavily reinforced sections in Slabs, Beams, Walls, Columns; Slip form work; Pumped Concrete. Medium 50-100 Trench fill; In-Situ Piling; Tremie Concrete High

8
**Degree of Site Control (Table 8, IS:456-2000) Good**

Site control having proper storage of cement; weigh batching of all materials; Controlled addition of water, regular checking of all materials, aggregate grading and moisture content; And periodical checking of workability and strength. Fair Site control having deviation from the above.

9
**Type of Exposure (Table 3, IS:456-2000)**

Sl. No. Environment Exposure Conditions 1 2 3 i) Mild Concrete surfaces protected against weather or aggressive conditions, except those situated in coastal area. ii) Moderate Concrete surfaces sheltered from severe rain or freezing whilst wet. Concrete exposed to condensation and rain. Concrete continuously under water. Concrete in contact or buried under non-aggressive soil/ground water. Concrete surfaces sheltered from saturated salt air in coastal area. iii) Severe Concrete surfaces exposed to severe rain, alternate wetting and drying or occasional freezing whilst wet or severe condensation. Concrete completely immersed in sea water. Concrete exposed to coastal environment. iv) Very Severe Concrete exposed to sea water spray, corrosive fumes or severe freezing conditions whilst wet. Concrete in contact with or buried under aggressive sub-soil/ground water. v) Extreme Surface of members in tidal zone. Members in direct contact with liquid/solid aggressive chemicals.

10
**Approximate Quantity of Materials required for concrete mix design**

Cement : 200 Kg. Fine Aggregate : 240 Kg. Coarse Aggregate : 180 Kg. (20 mm) 180 Kg. (10 mm)

11
**STEPS INVOLVED IN CONCRETE MIX DESIGN**

Step I:- Determine the physical properties of concrete ingredients. I. CEMENT (OPC 43 Grade) Sl. No. Particulars of Test Result Specifications As per IS: 1 Standard consistency (% by weight) 25.6 2 Setting Time in minutes a) Initial b) Final 95 210 30 Minimum 600 Maximum 3 Compressive Strength in N/sq.mm at the age of a) 3 days b) 7 days c) 28 days 24 35 46 23 Minimum 33 Minimum 43 Minimum 4 Specific Gravity 3.00 5 Fineness in Sq.m/Kg 337 225 Minimum

12
**Specifications for Zone–II**

FINE AGGREGATE 1. Sieve Analysis Sieve Size % Passing Specifications for Zone–II As per IS: 10.0 mm 100 4.75 mm 90-100 2.36 mm 98 75-100 1.18 mm 65 55-90 600 micron 42 35-59 300 micron 8 8-30 150 micron 0-10 2. Specific Gravity : 2.60 3. Unit Weight in Kg/Cu.m a) Loose : 1460 b) Rodded : 1580 4. Materials Finer than 75 micron : Max (% by weight)

13
**III. 20.0mm COARSE AGGREGATE 1. Sieve Analysis**

Sieve Size % Passing Specifications As per IS: Graded Single Sized 40.00mm 100 20.00mm 90 95-100 85-100 10.00mm 3 25-55 0-20 4.75mm 0-10 0-5 2. Specific Gravity : 2.65 3. Unit Weight in Kg/Cu.m a) Loose : 1467 b) Rodded : 1633

14
**IV. MECHANICAL PROPERTIES**

Sl. No. Particulars of Test Result Specifications As per IS: 1 Crushing Value in % 28 30 Maximum For wearing surfaces 45 Maximum For other concrete 2 Impact Value in % 24 3 Los Angeles Abrasion Value in % 30 50 Maximum

15
**V. 10.0mm COARSE AGGREGATE 1. Sieve Analysis 2. Unit Weight in Kg/Cu.m**

Sieve Size % Passing Specifications As per IS: Graded Single Sized 12.50mm 100 – 10.00mm 85 85-100 4.75mm 19 0-20 2.36mm 0-5 2. Unit Weight in Kg/Cu.m a) Loose : 1427 b) Rodded : 1587

16
**VI. BLENDING OF COARSE AGGREGATE:**

Sieve size (mm) IS: Specifications (Graded) % Passing 20 mm 10 mm 60%+40% 50%+50% 40 100 20 95-100 90 94 95 10 25-55 3 85 44 4.75 0-10 19 7

17
**Step II:- Compute Target Mean Compressive Strength:**

Fck = fck + t * S Fck = Target Mean Compressive Strength at 28 days in N/Sq.mm fck = Characteristic Compressive Strength at 28 days in S = Standard Deviation in N/Sq.mm t = A Statistic, depending on accepeted proportion of low results. = for 1 in 20 accepted proportion of low results

18
**Accepted proportion of low results**

Values of t Accepted proportion of low results t 1 in 5, % 0.84 1 in 10, 10% 1.28 1 in 15, % 1.50 1 in 20, 5% 1.65 1in 40, % 1.86 1 in 100, 1% 2.33

19
**Assumed Standard Deviation**

(Table 8, IS: ) Grade of Concrete Assumed Standard Deviation (N/Sq.mm) Good Site Control Fair Site Control M10, M15 3.5 4.5 M20, M25 4.0 5.0 M30, M35 M,40,M45 M50 6.0

20
**Step III:- Select the Water-Cement ratio of trial mix from experience**

No. Concrete Grade Minimum expected W/C 1 M10 0.9 2 M15 0.7 3 M20 0.55 4 M25 0.50 5 M30 0.45 6 M35 0.40 7 M40 0.35 8 M45 0.30

21
**Maximum size of Aggregate Water Content per cubic metre of concrete**

Step IV:- Select the water content per cubic metre of concrete from table2 of I.S: Maximum size of Aggregate (mm) Water Content per cubic metre of concrete (Kg) 10 208 20 186 40 165

22
**Maximum Size of Aggregate**

Approximate water content (Kg) per cubic metre of concrete (Table 32, SP: ) Slump (mm) Maximum Size of Aggregate 10 20 40 30-50 205 185 160 80-100 225 200 175 240 210

23
**Volume of Coarse Aggregate per Unit Volume of Total Aggregate**

(Table 3, IS: ) Maximum Size of Aggregate (mm) Volume of Coarse Aggregate per Unit Volume of Total Aggregate Zone IV Zone III Zone II Zone I 10 0.50 0.48 0.46 0.44 20 0.66 0.64 0.62 0.60 40 0.75 0.73 0.71 0.69

25
**Step V:- Compute the quantity of cement as follows.**

Water Cement = W/C Ratio = 185 / 0.45 = 411 Kg.

26
**Step VI:- Then we find the quantities of Fine & Coarse aggregate by absolute volume method.**

V = (W+C/Sc+(1/p) * (fa/Sfa)) * (1/1000) (Eq.1) and V = (W+C/Sc+(1/(1-p)) * (ca/Sca)) * (1/1000) (Eq.2) Where V = Absolute volume of fresh concrete = 1 m3 W = Mass of Water (Kg) per m3 of concrete C = Mass of Cement (Kg) per m3 of concrete p = Percentage of fine aggregate. fa = Mass of fine aggregate ca = Mass of coarse aggregate Sc = Specific gravity of cement. Sfa = Specific gravity of fine aggregate. Sca = Specific gravity of coarse aggregate.

27
**Substituting the values in Eq(1), we get**

1000 = /3.0 + (1/0.36) * fa /2.6) = fa/0.936 = fa/0.936 fa = (1000 – 322) * 0.936 = 678 * 0.936 = 635 Kg.

28
**Substituting the values in Eq(2), we get**

1000 = /3.0 + (1/0.64) * ca /2.65) = ca/1.696 = ca/1.696 ca = (1000 – 322) * 1.696 = 678 * 1.696 = 1150 Kg.

29
**So the mix proportion works out to be**

W : C : fa : ca = 185 : 411 : 635 : 1150 = : 1 : 1.55 : 2.80 This mix will be considered as Trial Mix No.2

30
**Step VII:- Make slump trials to find out the actual weight of water**

to get required slump. Make corrections to the water content & %FA, if required. Step VIII:- Compute 2 more trial mixes with W/C ratios as 0.40 & 0.50, taking %FA as 34% and 38% respectively.

31
Trial Mix No. 1:- Cement = 185 / 0.4 = Kg. Substituting the values in Eq(1), we get 1000 = /3.0 + (1/0.34) * fa /2.6) fa = 584 Kg. Substituting the values in Eq(2), we get 1000 = /3.0 + (1/0.66) * ca /2.65) ca = 1156 Kg. So the mix proportion works out to be W : C : fa : ca = 185 : : 584 : 1156 = 0.4 : 1 : 1.26 : 2.50

32
Trial Mix No. 3:- Cement = 185 / 0.5 = 370 Kg. Substituting the values in Eq(1), we get 1000 = /3.0 + (1/0.38) * fa /2.6) fa = 683 Kg. Substituting the values in Eq(2), we get 1000 = /3.0 + (1/0.62) * ca /2.65) ca = 1136 Kg. So the mix proportion works out to be W : C : fa : ca = 185 : 370 : 683 : 1136 = 0.5 : 1 : 1.85 : 3.07

33
**Step IX:- Cast atleast 3 cubes for each trial mix.**

Step X:- Test the cubes for compressive strength at 28 days.

34
**28 Days Compressive Strengths of Trial Mixes**

W/C Ratio C/W Ratio Compressive Strength (Kg/Cm2) 0.40 2.50 457 0.45 2.22 420 0.50 2.00 360

35
**Step XI:- Draw a graph between compressive strength Vs C/W Ratio.**

37
**Step XII:- From the graph, find the W/C ratio for the required**

target mean compressive strength. Step XIII:- Calculate the mix proportions corresponding to the W/C ratio, obtained from the graph.

38
Final Mix:- From the graph, for a target strength of 390 Kg/Cm2, W/C ratio = 0.47 Cement = 185 / 0.47 = 394 Kg. Substituting the values in Eq(1), we get 1000 = /3.0 + (1/0.38) * fa /2.6) fa = 675 Kg. Substituting the values in Eq(2), we get 1000 = /3.0 + (1/0.62) * ca /2.65) ca = 1123 Kg. So the mix proportion works out to be W : C : fa : ca = 185 : 394 : 675 : 1123 = : 1 : 1.71 : 2.85

39
Step XIV:- Check the cement content & W/C ratio against the limiting values given in Table-5 of I.S: for given type of exposure & type of Concrete.

40
Table-5 Minimum Cement content Maximum Water-Cement ratio and Minimum Grade of Concrete for different exposures with normal weight of aggregate of 20mm nominal maximum size. Sl. No. Exposure Plain Concrete Reinforced Concrete Minimum Cement Content kg/m3 Maximum Free Water Cement Ratio Minimum Grade of Concrete i) Mild 220 0.60 - 300 0.55 M20 ii) Moderate 240 M15 0.50 M25 iii) Severe 250 320 0.45 M30 iv) Very Severe 260 340 M35 v) Extreme 280 0.40 360 M40

41
**The W/C Ratio = 0.47 < 0.5 Hence Ok**

From the table 5 of IS: 456–2000, the minimum Cement content & W/C ratio, For moderate, for RCC are 300Kgs. & 0.5 The Cement content = 394Kgs. > 300Kgs. Hence Ok The W/C Ratio = 0.47 < 0.5 Hence Ok

42
**Concrete Mix RCC M30 with 20.0mm M.S.A.**

TEST REPORT Concrete Mix RCC M30 with 20.0mm M.S.A. Sl. No. Particulars Result 1 Characteristic Compressive strength in N/Sq.mm 30 2 Maximum size of Aggregate in mm 20.0 3 Type of Exposure Moderate 4 Type of Site control Good 5 Target Average Compressive Strength in N/Sq.mm 38.2 6 Workability in terms of Slump in mm 25-75 7 Mode of Compaction Vibration 8 Mix Partiuclars: a. Water-Cement Ratio b. Materials per cubic metre of concrete in Kg. i) Water ii) Cement (OPC 43 Grade) iii) Fine Aggregate iv) Coarse Aggregate c. Mix Portion by weight 0.47 185 394 675 1123 1:1.71:2.85

43
Secondary Slides:

44
**Sieve Analysis of Fine Aggregate**

Weight of sample = 500g (approx) Observations: Sieve size Weight retained(g) Cumulative weight retained (g) % Cumulative weight retained (g) % Passing IS: Specifications Zone =II Trail 1 Trail2 Total 10 mm 100 4.75 mm 2 4 90-100 2.36 mm 6 7 13 17 98 75-100 1.18 mm 166 165 331 348 35 65 55-90 600 micron 118 117 235 583 58 42 35-59 300 micron 175 160 335 918 92 8 8-30 150 micron 36 78 996 0-10 150 micron pass -

45
**Zones of Fine Aggregate**

Sieve Size IS : 383 – 1970 % Passing for Zone I Zone II Zone III Zone IV 10.00 mm 100 4.75 mm 90-100 95-100 2.36 mm 60-95 75-100 85-100 1.18 mm 30-70 55-90 600 micron 15-34 35-59 60-79 80-100 300 micron 5-20 8-30 12-40 15-50 150 micron 0-10 0-15

46
**Sieve Analysis of Coarse Aggregate**

mm aggregate : a. Minimum weight of sample = 25 Kg b. Observations : Sieve size Weight retained (Kg) Cumulative weight retained (Kg) % Cumulative weight retained (Kg) % Passing IS: Specifications Graded Single sized 40 0.0 100 20 4.7 10 90 95-100 85-100 41.5 46.2 97 3 25-55 0-20 4.75 1.6 47.8 0-10 0-5 4.75 P -

47
**Sieve Analysis of Coarse Aggregate**

mm aggregate : a. Minimum weight of sample = 12 Kg b. Observations : Sieve size Weight retained (Kg) Cumulative weight retained (Kg) % Cumulative weight retained (Kg) % Passing IS: Specifications Single Sized 12.5 0.0 100 10 5.4 15 85 85-100 4.75 24.3 29.7 81 19 0-20 2.36 6.9 36.6 0-5 2.36 P -

48
**Target mean compressive strength**

Avg = 30 Avg = 35 27,30,30,32,35, 27,33,34,29,28, 30,28,31,32,26, 34,33,25,27,29 28, 32,35,38,40, 34,35,35,36,39, 33,32,32,34,37, 32,35,38,39,36 Total = 600 Total = 700

49
The value of ‘S’ depends on Degree of Site control and grade of concrete as given in I.S: 456–2000 (Table.8) Sl. No. Concrete Grade Good Fair S 1.65XS Fck N/mm2 Kg/cm2 1 M10 3.5 58 15.8 161 4.5 7.4 17.4 178 2 M15 20.8 212 22.4 229 3 M20 4.0 6.6 26.6 271 5.0 8.3 28.3 288 4 M25 31.6 322 33.3 339 5 M30 38.3 390 6.0 9.9 39.9 407 6 M35 43.3 441 44.9 458

50
**Step IV:-Fixation of Water Cement ratios for trial mixes.**

Sl. No. Required Grades Trial W/C 1 M20, M15, M10 0.55, 0.6, 0.9 2 M25, M20, M15 0.5, 0.6, 0.7

51
Final Mix for RCC-M25:- From the graph, for a target strength of 322 Kg/Cm2, W/C ratio = 0.57 which is > 0.5, So, limit W/C ratio to 0.5 only. Cement = 185 / 0.5 = 370 Kg. Substituting the values in Eq(1), we get 1000 = /3.0 + (1/0.38) * fa /2.6) fa = 683 Kg. Substituting the values in Eq(2), we get 1000 = /3.0 + (1/0.62) * ca /2.65) ca = 1136 Kg. So the mix proportion works out to be W : C : fa : ca = 185 : 370 : 683 : 1136 = : 1 : 1.85 : 3.07

52
**Specific Gravity of Cement [ IS : 4031 – 1988]:**

Specific gravity of cement (Sc) (W2 - W1) = x 0.79 (W4 - W1) - (W3 - W2) Where, W1 = Weight of specific gravity bottle in g W2 = Weight of specific gravity bottle with about half filled cement in g W3 = Weight of specific gravity bottle with about half filled cement & rest is filled with kerosene in g. W4 = Weight of specific gravity bottle completely filled with kerosene in g 0.79 = Specific Gravity of Kerosene.

53
**Specific Gravity of Fine Aggregate & Coarse Aggregate [ IS : 2386 (Part.3) - 1963]:**

D Specific gravity (Gs) = C – ( A – B) Where, A = Weight of Pycnometer vessel containing sample & filled with distilled water in g B = Weight of Pycnometer completely filled with distilled water only in g C = Weight of saturated surface dry sample in g D = Weight of oven dried sample in g

55
Thank You

Similar presentations

Presentation is loading. Please wait....

OK

CEMENT CONCRETE MIX DESIGN

CEMENT CONCRETE MIX DESIGN

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on acid-base indicators worksheets Download ppt on folk dances of india Ppt on lean production system Ppt on media revolution Ppt on world diabetes day 2015 Ppt on democratic and non democratic countries Ppt on water scarcity in the middle east Ppt on satellite orbit calculator Ppt on object-oriented technologies Ppt on summary writing sample